1 UNECE United Nations Economic Commission for Europe Food and Agriculture Organization of the United Nations GENEVA TIMBER AND FOREST DISCUSSION PAPER 49 FOREST PRODUCT CONVERSION FACTORS FOR THE UNECE REGION UNITED NATIONS
3 United Nations Economic Commission for Europe/ Food and Agriculture Organization of the United Nations UNECE ECE/TIM/DP/49 Timber Section, Geneva, Switzerland GENEVA TIMBER AND FOREST DISCUSSION PAPER 49 FOREST PRODUCT CONVERSION FACTORS FOR THE UNECE REGION UNITED NATIONS Geneva, 2010
4 Note The designations employed and the presentation of material in this publication do not imply the expression of any opinion whatsoever on the part of the secretariat of the United Nations concerning the legal status of any country, territory, city or area, or of its authorities, or concerning the delimitation of its frontiers or boundaries. Abstract Forest Product Conversion Factors for the UNECE Region provides ratios of raw material input to the output of wood-based forest products for sixteen countries of the UNECE region. Analysts, policymakers, forest practitioners and forest-based manufacturers often have a need for this information when looking into the future of the forest sector via outlook studies, but also for a basic understanding of the drivers of efficiency, feasibility and economics of the sector. The publication includes explanations on the units of measure, the drivers of the ratios, as well as information on physical properties of wood-based forest products. Finally, where reported factors were unavailable, factors from other sources are given. Keywords Conversion factors, fibreboard, forest products, house logs, lumber, logs, OSB, particleboard, plywood, panels, pulp and paper, pilings, physical properties, poles, posts, ratio, recovery, roundwood, sawnwood, shakes, shingles, staves, veneer, wood energy, wood particles, wood pellets ECE/TIM/DP/49 UNITED NATIONS PUBLICATION ISSN
5 Forest products conversion factors for the UNECE Region iii Preface The collection and reporting of conversion factors by UNECE/FAO has been done at least eight times previously; starting in 1963, with the last formal report published in Given the changes that have occurred in the forest sector since the last report, it was timely of the FAO/UNECE Working Party on Forest Economics and Statistics to request this task. Two key mandates of the UNECE/FAO Timber Section which use conversion factors are the regular reporting, analysis and dissemination of UNECE region forest products statistics and to conduct periodic assessments of the forest sector outlook within the region. Conversion factors are also important for benchmarking manufacturing efficiency, conducting trade in wood products and analyzing the feasibility of many transactions and business processes. While it would appear that simply asking countries and practitioners for their list of conversion factors would be a simple process, it is complex as a result of the myriad of measurement unit definitions, utilization standards, measurement procedures, manufacturing practices, and the variability that is inherent in making diverse products from trees, which vary in size, shape, and density. This report has gone beyond what was done in the past by providing insight into the drivers of product recovery factors and explanations as to why conversion factors vary. Subregional differences in measurement standards and factors have also been pointed to in the hope that further investigation and cooperation will improve harmonization of data and factors. This has a bearing not only on conversion factors, but also on nationally reported forest products statistics. The report provides analysts, forest practitioners and private enterprises with the most current forest product conversion factors available and a better understanding of the units used in the manufacture, trade and reporting of wood-based forest products. Finally, this report will provide all in the intended audience with a better ability to understand the future outlook for the forest sector, estimate manufacturing efficiency and convert between units of measure within our region. I express my appreciation to the Task Force, the national experts and the secretariat for this timely publication. Ján Kubiš Executive Secretary United Nations Economic Commission for Europe
6 iv Forest products conversion factors for the UNECE Region Acknowledgements The secretariat of the UNECE/FAO Timber Section wish to thank all of the members of the Task Force who assisted with this project. The Task Force members are: Pekka Alajarvi, Stora Enso, Finland Wolfgang Bittermann, Statistik Austria Lars Bjorklund, Swedish Timber Measurement Council* Filip De Jaeger, European Organization of the Sawmill Industry, Belgium Peder Gjerdrum, Norwegian Forest and Landscape Institute* Peter Ince, United States Department of Agriculture, Forest Service, United States of America* Romain Jacques, Natural Resources Canada* Dmitriy Katkov, Russian Federal Forest Agency Eric Kilby, Confederation of European Paper Industries, Belgium* Arvydas Lebedys, Food and Agriculture Organization of the United Nations, Italy Nico Leek, Probos, Netherlands* Udo Mantau, University of Hamburg, Germany Eoin O'Driscoll, Council for Forest Research and Development, Ireland* Tatiana Pasi, Swiss Federal Office for the Environment, Switzerland* Susan Phelps, Natural Resources Canada Juan Picos Martin, Monte Industria, Spain* Peter Schwarzbauer, University of Natural Resources and Applied Life Sciences, Austria* Henry Spelter, United States Department of Agriculture, Forest Service, United States of America* Roman Svitok, National Forest Centre, Slovakia* Michal Synek, Forest Management Institute, Czech Republic* Alain Thivolle-Cazat, Institut Technique Forêt Cellulose Bois-Construction Ameublement, France* Erkki Verkasalo, Finnish Forest Research Institute* Darius Vizlenskas, State Forest Service, Lithuania* Sheila Ward, Forestry Commission, United Kingdom* Holger Weimar, Federal Research Institute for Rural Areas, Forestry and Fisheries, Germany* Adrian Whiteman, Food and Agriculture Organization of the United Nations, Italy Note: *Indicates that this Task Force member also filled in the questionnaire for their country, or for a sector within a country that their organization represents. The work of the Task Force and the production of this publication were supported by the following members of the Geneva-based UNECE/FAO Timber Section: Douglas Clark Matt Fonseca Alex McCusker Ed Pepke Christopher Prins Florian Steierer Many thanks to all of the people listed above for their contribution of time and expertise. Anyone having relevant information on forest products conversion factors, which could be used to improve future revisions of this publication are invited to contact the UNECE/FAO Timber Section. Matt Fonseca, Project Leader UNECE/FAO Timber Section Trade and Timber Division United Nations Economic Commission for Europe Palais des Nations CH-1211 Geneva 10 Switzerland
7 Forest products conversion factors for the UNECE Region v Preface Acknowledgements List of Abreviations C O N T E N T S Page... iii...iv...vii INTRODUCTION...1 Conversion factors general use...2 Conversion factors use by UNECE/FAO...2 Methods ROUNDWOOD Volumetric measurement Cubic volume Board foot log rules Stacked measure Weight and physical properties Wood density Moisture content Bark and other unmeasured volume Summary of country data on roundwood WOOD PARTICLES Volumetric measurement Weight Summary of country data on wood particles SAWNWOOD Volumetric measurement Cubic volume Board foot volume Weight Material balance Summary of country data on sawnwood VENEER AND PLYWOOD Volumetric and surface measurement Weight Material balance Summary of country data on veneer and plywood PANELS MADE OF WOOD PARTICLES Volumetric and surface measurement Weight...20 Summary of country data on panels made from wood particles WOOD PULP AND PAPER Weight...22 Summary of country data on wood pulp and paper ROUND AND SPLIT WOOD PRODUCTS Volumetric and surface measurement Weight Material balance Summary of country data on round and split wood products ENERGY WOOD PRODUCTS AND PROPERTIES Volumetric measurement Weight Energy values Summary of country data on energy wood products and properties REFERENCES...27 ANNEX...29
8 vi Forest products conversion factors for the UNECE Region List of figures Page 1.1 True log volume calculation Log volume comparison between national log scales for log in figure Board foot log rules by small-end diameter class indexed against 1 m 3 of B.C. Firmwood Example of roundwood to sawnwood factors by state of manufacture Material balance and sawnwood recovery by small-end diameter Material balance in the sawmilling process for coniferous sawnwood Material balance in the sawmilling process for non-coniferous sawnwood Material balance and rotary peeled plywood recovery by small-end diameter...18 Annex figure 1 Example of wood balance using conversion factors...30 List of tables Page 1.1 Swedish National Board of Forestry stacked measure guidelines for pulp logs Summary of country data on roundwood Summary of country data on wood particles Board foot actual to nominal sizes and volumes by lumber (sawnwood) product type Summary of country data on sawnwood Summary of country data on veneer and plywood Summary of country data on panels made from wood particles Summary of country data on wood pulp and paper Summary of country data on round and split wood products Summary of country data on energy wood products and properties...26 Annex tables 1 List of equivalents Joint Forest Sector Questionnaire Conversion Factors Conversion factors used in the European Forest Sector Outlook Study Country groupings with similar forest product sectors Conversion factors from ECE/TIM/
9 Forest products conversion factors for the UNECE Region vii List of abbreviations AB Alberta BC British Columbia bf board foot or board feet C Celsius cm centimetre FAO Food and Agriculture Organization of the United Nations GOST Government standard of the Russian Federation ft foot or feet ft 2 square foot gj gigajoule gm gram kl kilolitre kg kilogram lbs pounds m metre m 2 square metre m 3 cubic metre m 3 p cubic metre product m 3 rw cubic metre roundwood m 3 sw cubic metre of solid wood mbf 1,000 board feet mcd moisture content dry basis mcw moisture content wet basis MDF medium density fibreboard mm millimetre mt metric ton n.a. not applicable NWLRAG Northwest Log Rules Advisory Group ob over bark odmt oven dry metric ton OSB oriented strand-board RW roundwood swe solid wood equivalent ub under bark UNECE United Nations Economic Commission for Europe USFS United States Department of Agriculture, Forest Service
11 Forest products conversion factors for the UNECE Region 1 INTRODUCTION The origins of this paper lie in a workshop, National Wood Energy Resource Balances, held in Geneva on 31 March and 1 April A background paper, Conversion Factors: A Necessity for an Accurate Estimation of Wood Consumption by Industries 1 (Thivolle-Cazat, 2008) highlighted the varied approaches to estimating roundwood consumption based on the outputs of wood products, as well as the challenge to convert these varied data into harmonized international units, which may then be compared directly. The challenge is certainly not new. The Joint FAO/UNECE Working Party on Forest Economics and Statistics has been concerned with the problem of raw material/product conversion factors since the 1950s. It instituted a system of regular monitoring and reporting of national forest product conversion factors. However, the most recent report prior to this one was done in The 2008 Joint FAO/UNECE Working Party, meeting immediately after the workshop, mandated the UNECE/FAO Timber Section to lead a cooperative effort to develop accurate conversion factors for the UNECE region as an aid to establishing national and subregional wood balances. The result was the establishment of a Task Force of national and industry-based experts, which met for the first time on June 2008 in Geneva 2. This paper describes the method adopted by the Task Force to arrive at a set of conversion factors. It presents the results of its work and then summarizes and compares the conversion factors by products for the countries that responded to a questionnaire enquiry. The term forest products conversion factors is used to cover a broad spectrum of ratios utilized in the woodbased forest resource, manufacturing, and energy sectors. For the purpose of this publication, conversion factor is defined as using a known figure to determine or estimate an unknown figure via a ratio. Often these ratios are exact, for example converting cubic feet to cubic metres (there is exactly cubic feet in a cubic metre). Annex table 1 is a listing of some of the exact conversion factors (equivalents) relevant to forest products. Often ratios are not exact, but rather a good average; for example, a cubic metre (under bark volume) of freshly felled Norway spruce sawlogs may average 860 kg of which 80 kg is bark and 780 kg is wood (with both bark and wood containing a certain amount of moisture), but might vary as a result of wood density, moisture content, the presence or lack of bark, etc. In other instances, conversion factors may have little meaning unless some of the parameters of the numerator and the denominator of the ratio are known. For example: a cubic metre of logs with an average small end diameter of 15 cm might make 0.41 m 3 of sawnwood, while a cubic metre of logs with an average small-end diameter of 60 cm might make 0.63 m 3 (50% more), given the same level of processing efficiency in a sawmill. That is not to say that a single factor to convert roundwood to sawnwood cannot be used; it can be done with an accurate factor and when looking at a large population in the aggregate. When looking at a lower level, however, factors that account for various parameters are better suited (e.g. a mill or a subregion that only processes small logs). Related to forest product conversion factors, is the use of the material balance (see annex figure 1). The sawnwood example above could lead to the incorrect assumption that only 41% of the wood fibre in the 15 cm sawlog and 63% of the 60 cm sawlog were utilized. In fact, almost 100% of the wood in each of these logs may have been utilized. The remaining non-sawnwood volume went to several wood residues having other and often distinct uses. For example: a cubic metre of 15 cm sawlogs could have a material balance of 41% sawnwood, 43% chips (raw material for paper, panels, wood energy, etc.), 9% sawdust (for making energy pellets, particleboard, MDF, etc.) and finally 7% shavings (particle board, MDF, animal bedding and wood energy, etc.). The components balance with 100%. Although not part of the material balance, as the log volume was represented as under bark, one might also apply a conversion factor to this scenario to estimate that 80 kg of bark (with moisture) are potentially available from each cubic metre of roundwood (measured under bark) for energy or other uses. Note that material balances are used at a manufacturing plant level, a sector level, or can be constructed to account for the cascading uses of wood raw material in a country, subregion, or region (Mantau, 2008). 1 Available at: 2 Minutes of the meeting are available at:
12 2 Forest products conversion factors for the UNECE Region Logs and their subsequent products have a predisposition towards inexact conversion factors, as a result of the wide range of shape and form, the variability of physical properties (density, moisture content and shrinkage), and other natural variables that affect conversion factors, such as species, size, defects or provenance. Wood fibre is also hygroscopic, thus its volume and weight change once dried in a kiln or exposed to the atmosphere. In addition, there are external biases that also have to be accounted for, such as differences in measurement procedures which often reflect a unit volume differently than another standard does. Finally, there are differences that occur as a result of product-manufacturing efficiency levels and utilization practices. Conversion factors general use Conversion factors have long been utilized by the forest sector as a tool for analysing forests and forest products manufacturing facilities. Virtually every aspect of forecasting and analysis in the forest sector is somehow touched by conversion factors. Silvicultural growth models, biomass calculations, carbon sequestered in the forest, timber sale appraisals, to name just a few, are all dependent on conversion factors. A practical example of this would be a timber sale appraisal that a sawmill is conducting to determine a bid price. The stand volume may be reported in cubic metres over bark but the purchaser may need to convert these volumes into inside bark volumes, weight or board feet 3 to match their units of measure. To determine the value of the timber, the purchaser will need to know the cost of getting the timber from the stump to the mill site, thus weight to volume ratios are likely to be an important parameter for determining weight-based transport costs. Primary product recovery will need to be estimated using conversion factors from roundwood to the primary product, e.g., 2 m 3 roundwood will produce 1 m 3 sawnwood. A material balance will be used to determine the quantity and thus value of the residual products made, and finally, ratios may be used to estimate the quantity of unmeasured products from the timber sale such as bark and logging residue (top-wood, limbs, foliage) which may be profitable to utilize for energy or other purposes. Analysts have used conversion factors in an effort to try to indicate illegally logged roundwood in the supply chain of manufacturing facilities in a subregion, i.e. when the roundwood removal volume is less than the apparent consumption as determined via conversion factors, it is assumed that the disparity may be made up of illegally logged volume. Additionally, organizations including the Convention on International Trade in Endangered Species (CITES) and others have been looking into the possibility of applying conversion factors to manufactured product volumes as an indication of the harvest level of endangered species such as bigleaf mahogany (CITES, 2008). Conversion factors covering the input of raw material to output of forest products are a good indication of efficiency levels and thus are often used to benchmark a manufacturing facility s effectiveness at converting raw materials into finished or semi-finished products. At a higher level, policy analysts and policymakers may utilize conversion factors to determine the sequestered carbon in the forests of their country. The recent trade disputes and subsequent agreements on sawn softwood between the United States and Canada used conversion factors for comparing stumpage prices between the two countries (World Trade Organization, 2003). Finally, outlook studies on long-term wood availability depend on conversion factors to predict needed raw materials to match the forecasted demand of wood and paper products. Conversion factors use by UNECE/FAO To quote directly from Conversion Factors (Raw Material/Product) for Forest Products, (UNECE/FAO, 1987) 4 : A major objective of collecting and publishing this information on an international basis is to calculate national and international wood balances, notably in the context of the UNECE/FAO studies of European timber trends and prospects, in order to estimate wood requirements. This information is also of use in the preparation of other national and international studies with a wood balance element. 3 A board foot is ostensibly the equivalent volume of a board that is 1 inch thick x 1 foot wide x 1 foot long ( m 3 ). 4 The publication is available at:
13 Forest products conversion factors for the UNECE Region 3 At the data collection level, conversion factors for the following are also utilized: 1. Where a country has explicitly provided data in non-standard units. Typically this involves a conversion from square metres to cubic metres or from metric tons to cubic metres. Conversion factors from FAO are used for the metric tons to cubic metres. For the square metres to cubic metres conversion of panels, an estimate of the average thickness of the type of panels is needed (see annex table 2), Joint Forest Sector Questionnaire conversion factors sheet). 2. Where it is suspected that data are incorrect. Often the unit value (dividing value of trade of a product by its volume of trade) will indicate that an element is incorrect. Most obviously, plywood and fibreboard data are often reported in square metres rather than cubic metres without this being explicitly stated. Here, a standard unit value (e.g. an average thickness) is applied to convert the area figure into volume. 3. Converting data from other sources to UNECE/FAO standards (e.g. UN Comtrade 5 data reported in kilograms). Official trade statistics usually indicate a trade volume in kilograms. Other units are also used but these are often not consistently applied. Thus when extracting data from UN Comtrade, for example, the total of the weight is converted from metric tons to m 3 using the FAO standard conversion factors. Clearly defining units used for harmonization is also an area that has been identified as important for the UNECE/FAO. Not only because it is necessary for obtaining accurate conversion factors, but also for understanding volumes when comparing national statistics, e.g. is a cubic metre of roundwood or sawnwood as reported from one country volumetrically equivalent to that from another country. Conversion factors were used for the European Forest Sector Outlook Study, which was published in 2005 (UNECE, 2005) (see annex 3 for the conversion factors used). Moreover, forest product conversion factors have been a topic of work by the UNECE/FAO Timber Section on National Wood Resource Balances (March 2008) 6. Methods The Task Force reviewed the current problems with existing conversion factors and finalized the units and definitions as well as the desired factors and balances of the various forest products. It also categorized the countries of the UNECE region into 19 groups that were expected to have similar conversion factors (annex table 4). This list is intended to be used to fill a void in information from a country by using the data of another country from the same group. Unfortunately, there are some country groupings without a single country represented by responses to this study s inquiry. In lieu of other sources; annex table 3 includes the conversion factors used for the European Forest Sector Outlook Study : Main Report 7 (UNECE/FAO, 2005) and annex table 5 includes the conversion factors from Conversion Factors for Forest Products, (UNECE/FAO, 1987). A questionnaire was developed 8 and distributed to the Task Force members as well as to other national correspondents for collection of national conversion factors. The last of the completed questionnaires was received in January Sixteen countries and one trade association submitted conversion factors 9. 5 The UN Commodity Trade Statistics Database is available at: 6 Documentation from this workshop is available at: 7 This table is available at: 8 The questionnaire is available at: 9 Austria, Canada, Czech Republic, Finland, France, Germany, Ireland, Lithuania, Netherlands, Norway, Slovakia, Spain, Sweden, Switzerland, United Kingdom, United States of America, and the Confederation of European Paper Industries.
14 4 Forest products conversion factors for the UNECE Region 1. ROUNDWOOD The conversion factors requested in the questionnaire related to two areas: 1. physical properties; and 2. national method of measuring roundwood as it relates to the true volume. Note that true volume of roundwood for the purposes of this publication and for UNECE/FAO statistics on roundwood volume always means under bark volume. Conversion factors for roundwood are often used to convert from one unit of measure to another, e.g., from weight to volume. Additionally, conversion factors within the same units are also quite common, e.g. a cubic metre of roundwood measured by the national standard in one country may be different if measured by the national standard of another country. Most countries were able to submit data on the conversion factors relating to general physical properties of roundwood. It is important to note that species-specific data was not asked for; data fields were limited to coniferous and non-coniferous, with separate fields for saw and veneer logs, and pulp and energy logs. Data availability on conversion factors for harmonizing national standards of roundwood measurement to a true volume was somewhat limited, (see sections and 1.1.2). 1.1 Volumetric measurement Cubic volume Assessing the volume of roundwood is typically referred to as log scaling. In general, log scales attempt to either predict the displaced volume of the log (cubic log scale), or as is the case in the United States and some regions of Canada, in units of predicted output of sawnwood (board foot log rule). One of the questions asked in the questionnaire was: what is the ratio of volume as determined by your national standard to a m 3 of true volume? True volume was defined as the volume as determined using a logical cubic formula (one that approximates the volume of the log form) and unbiased rounding logic. There are a number of different cubic formulas, e.g. Smalian, Huber, Newton, centroid, or two-end conic, most with potential strengths and weaknesses which are dependent on log dimensions and form. All of the aforementioned cubic formulas will give similar results most of the time when measurement conventions are applied uniformly and on logs with typical parameters (figure 1.1). Thus, it is not within the scope of this report to specify a standardized roundwood volume formula. Figure 1.1 is an example of volume calculation using unbiased rounding logic and two different formulas (Smalian and Huber). Figure 1.1 True log volume calculation 5.02 m 23.2 cm 25.5 cm 28.1 cm 22.7 cm 25.3 cm 27.8 cm Smalian formula: ((( )/2) 2 +(( )/2) 2 ) x 5.02 x = 2.58 m 3 Huber formula: (( )/2) 2 x 5.02 x = 2.54 m 3 Source: UNECE/FAO, Of much greater concern, in terms of harmonizing conversion factors based on national volumes to true cubic, is the common practice of truncating (rounding down) diameters and lengths. For example: a log with an actual length of 10.3 metres is recorded as being 10.0 m in length (with 30 cm of unmeasured trim allowance ); and a log end with a diameter of 27.9 cm is recorded as having a diameter of 27.0 cm.
15 Forest products conversion factors for the UNECE Region 5 The purpose of truncation should not be construed as a purposeful way of understating volume; it is generally done to make the mathematical calculation easier and to allow the manufacture of products at least as long as the recorded log length. There are other areas that also create discrepancies between log scales, such as the reduction of volumes for defects vs. not accounting for defect with a volume reduction, but rather using a value reducing mechanism such as log grade. Additionally, some national and subregional log scaling standards treat the log as a cylinder with a diameter of the small-end of the log; assume the log form is a cylinder with the diameter that exists in the middle of the log length; or use assumed taper rates to establish diameters other than the small-end. Additionally, some national standards calculate the over bark volume. All of these differences can lead to variation in roundwood volume (figure 1.2). The figure shows saw/veneer log volumes calculated using thirteen different log scaling standards. Please note that this figure only represents one log and is included as an example of some of the differences that can occur. Logs with different dimensions and characteristics may produce quite different relative results, owing to the degree and points of rounding, as well as the relative size of truncated units, e.g. truncating a diameter of 13.9 cm to 13 will have a more significant impact to the volume on a percentage basis (-12.5%) then would truncating a diameter of 77.9 cm to 77 (-2.3%). While not included in the figure, the log shown in figure 1.1 would have a board foot volume of: 30 bf if measured in coastal Alaska, Oregon and Washington, US (Scribner long log rule). 40 bf if measured in the western US, except as noted above (Scribner short log rule). 25 bf if measured in the southeast of the US (Doyle log rule). 50 bf if measured in the northeast of the US (International ¼ inch log rule). 45 bf if measured in the province of Ontario, Canada (Ontario log rule). 48 bf if measured in the provinces of New Brunswick or Nova Scotia Canada (New Brunswick log rule). 54 bf if measured in the province of Newfoundland, Canada (Newfoundland log rule) Figure 1.2 Log volume comparison between national log scales for log in figure 1.1 Log volume (m 3 ) over bark over bark over bark % 14% 10% 6% 2% -2% -6% -10% -14% -18% -22% -26% -30% Difference from "true" Smalian (%) "True" Smalian "True" Huber Canada Alberta Canada British Columbia Finland France Ireland Germany Norway Russia GOST Sweden UK Conifer UK Hardwood US NWLRAG US Forest Service Note: Calculated using the log dimensions in figure 1.1 and applying the procedures from the national roundwood measurement standards from the countries or organizations listed. NWLRAG = Northwest Log Rules Advisory Group, GOST is the standard for domestically consumed roundwood in the Russian Federation, UK Conifer = top diameter method, UK Hardwood = mid diameter method. Source: See references under subsection on roundwood measurement standards (section 9.). For the purpose of this report, conversion factors using roundwood input are assumed to be based on true volume, which is what was requested in the questionnaire. It is known that many of the countries adjust their national roundwood measurement standard volume to a true volume for reporting, e.g. Finland, Sweden and the United States. This is an area where future study could improve the accuracy, comparability and harmonization of what is often the starting point (the numerator) for many of the forest product conversion factors used.
16 6 Forest products conversion factors for the UNECE Region Board foot log rules In the United States and in Canada there are still regions that use board foot log rules. Most of these rules date from the 19th century and attempt to predict sawnwood as measured in board feet which could be milled from a log. Log rules are either based on diagrams or formulas, with assumptions made as to saw kerf, and slab loss. Except for the International ¼ rule, log segments were considered to be a cylinder having no taper. A US study used a population of 175 logs to model the conversion factors of various board foot rules used in North America and found that the board foot per cubic metre 10, for just the Scribner rules (of which there are three subregional variants), ranged, on average, from as little as 108 (9.26 m 3 /1,000 board feet (mbf)) for logs with a small-end diameter of 4.5 to 7.49 inches to as much as 246 (4.06 m 3 /mbf) for logs with a small-end diameter over 15.5 inches (Fonseca, 2005). Figure 1.3 shows the conversion in mbf per cubic metre of the British Columbia standard (firmwood method) of measuring roundwood. As these rules do not correlate consistently with cubic volume across all diameters classes, it is necessary to view the ratios as they relate in various diameter groupings. In the past, many sources of published conversion factors (including those from UNECE/FAO) have used a universal 4.53 m 3 per mbf ratio (0.221 mbf/m 3 ) to convert mbf into m 3. This ratio dates from at least 1950 (Spelter, 2002) when timber harvest was concentrated on large diameter trees. Additionally, there is substantial subregional variation between the various board foot log rules and in the timber that they are applied to, so a subregional approach would appear to be more appropriate. In Conversion of Board Foot Scaled Logs to Cubic Meters in Washington State (Spelter, 2002), it was found that the conversion factor from Scribner long log mbf to m 3 had changed from about mbf/m 3 in 1970, to mbf in In the interior of the State (Scribner short log method), the ratio went from to mbf/m 3 during the same period). In the province of Nova Scotia, Canada, mbf/m 3 is used to convert logs measured with the board foot system to cubic metres. (Nova Scotia Department of Natural Resources, 2001). Figure 1.3 Board foot log rules by small-end diameter class indexed against 1 m 3 of B.C. Firmwood (mbf per m 3 BC Firmwood) Scribner Short (revised) Scribner Short (not revised) Scribner Long Log Doyle inches ( cm) inches ( cm) inches ( cm) >15.5 inches (>39.4 cm) International 1/4 inch Note: Board foot (bf) log rules indexed in units of 1,000 bf, e.g., 147 BF Scribner Short (revised) ( inch small end diameter) = 1.0 B.C. Firmwood m 3. This analysis is based on a control group of 175 logs. Scribner Short (revised) = revised rule used in California and interior Oregon and Washington; Scribner Short (not revised) = non-revised rule used outside of the Pacific coast states; Scribner Long Log used only in coastal Oregon, Washington, and Alaska; Doyle used primarily in the mid-west and southeast of the US; International ¼ inch used primarily in New England and eastern Canada. Source: Fonseca, The roundwood measurement standard of the province of British Columbia, Canada (B.C. Firmwood) was chosen as the index because it has unbiased rounding logic and uniform application of formulas and measurements.
17 Forest products conversion factors for the UNECE Region Stacked measure In the case of stacked roundwood, it is often assumed that approximately 66.7% of the displaced volume is wood, 11.5% is bark, and 21.6% is void. (Ontario Ministry of Natural Resources, 2000). In fact the ratio of wood volume can be less than 50% to more than 80% depending on many factors. A guideline to adjust for such factors can be found in Estimation of the Solid Volume Percentage (VMF Nord, 1999) shown in table 1.1, which allows estimation of the solid wood ratio based on visually assessed log attributes. Table 1.1 Swedish National Board of Forestry stacked measure guidelines for pulp logs Starting value 60% Average log diameter under bark Trimming of knots and buttress <8.99 cm - 4% Very well trimmed, few buttresses 0% cm -3% A few knot stumps and buttresses -1% cm -2% Many knot stumps and buttresses -2% cm -1% Many large knot stumps, clusters and buttresses -3 to 4% cm 0% Very bad trimming -5 to 7% cm +1% cm +2% Crookedness cm +3% Straight softwood, straight aspen 0 to-1% cm) +4% Crooked softwood, straight deciduous wood -2 to 3% cm +5% Very crooked softwood, crooked deciduous wood -4 to 5% cm +6% Very crooked deciduous wood -6 to 7% cm +7% Extremely crooked deciduous wood -8 to 12% cm +8% >27 cm +9% Bark volume Debarked wood +7% Quality of stacking More than ⅔ thin bark +2% Very good 0% More than ⅓ thin bark +1% Good -1% Normal conifer 0% Fair -2% Softwood with thick bark, normal deciduous bark -1% Bad -3 to -4% More than 50% deciduous wood with thick bark -2% Very bad -5 to -7% Source: VMF Nord, Weight and physical properties The weight of roundwood generally correlates well with the volume. In many areas of the world, roundwood is bought and sold via weight. Usually weight is used in conjunction with sample volume measurement in order to establish the relationship. The presence of drive-on weight scales along many transportation routes, national ports of entry, and at many industries that consume roundwood, make this data readily available and inexpensive to ascertain relative to taking measurements on all logs. There are a number of factors which determine the weight of a given amount of roundwood volume Wood density Wood is structured with cell walls and void spaces. Wood cell walls all have about the same basic density, regardless of species, approximately 1,560 kg per m 3, (Van Vuuran, et al. 1978). What varies is the amount of wood material to cell cavity area. Wood density is typically measured as a ratio of the weight of oven dry fibre per m 3 (basic density), or in the unitless measure of specific gravity, which is an index of the relationship of said material to the same volume of water (water weighs 1,000 kg/m 3 ). For example, a cubic metre of wood (volume measured when green), without any water weighs 400 kg; it has a basic density of 400 kg/m 3 and a specific gravity of In the UNECE region basic density (green volume and oven dry weight) will vary from approximately 290 kg/m 3 to 540 kg/m 3 for coniferous wood, while non-coniferous will vary from about 320 kg/m 3 to 800 kg/m 3 (USDA Forest Service, Forest Products Laboratory, 1999) and (Austrian Energy Agency, 2009).
18 8 Forest products conversion factors for the UNECE Region When using published averages for calculating the basic density or specific gravity of a species, be careful to note whether the volume was established in the green state (prior to shrinkage) or in the dry state (after shrinkage), as wood volume in the UNECE region will shrink approximately 10% for coniferous species and about 15% for hardwood species when taken from green to a fully dry state. The exact amount of shrinkage will vary from one species to another and even from one sample of the same species to another. In general, basic density based on green volume, which is the standard for this publication unless otherwise noted, has the advantage of being applicable to standing tree volume and roundwood without having to know or estimate volumetric shrinkage Moisture content Freshly cut wood contains large amounts of water, both in the cell cavities (free water) and within the cell walls themselves (bound water). Normally the moisture content is measured in terms of the weight of the moisture relative to the weight of the dry wood fibre. For example, if wood weighs 812 kg/m 3 in the green state, and 400 kg m 3 in the oven dry state (devoid of moisture), it is said to have 103% moisture content dry basis (mcd). In this example the wood had 400 kg of wood and 412 kg of moisture. Therefore, dividing the weight of the moisture by the weight of the dry wood gives the moisture content. Note that freshly cut wood can vary from 30% mcd to more than 200% mcd (USDA Forest Service, Forest Products Laboratory, 1999). Moisture content can also be reflected via the ratio of moisture weight to the total weight of the wood fibre plus moisture content, which is referred to as moisture content wet basis (mcw), but this is typically used for measuring the moisture content of wood particles, wood for energy, and pulp and paper, which will be elaborated upon further in sections 2 and 6. This method is not normally used for solid wood, as the numerator is made up partly by the denominator. It is also important to note that the moisture content of the wood and bark of many species has distinct seasonal variation. Some species may have little variation, while others may have significantly higher moisture content during the winter and early spring as opposed to the summer and early fall (Thivolle-Cazat, 2008). Finally, the heartwood of many species, particularly coniferous trees, often have less moisture than the sapwood. Thus, older (generally larger) trees often have a lower weight to volume ratio than that of younger trees (generally smaller) by virtue of the age related increase in the ratio of heartwood to sapwood. Related to this, many species have a higher ratio of bark when young and small vs. old and large, thereby magnifying this trend Bark and other unmeasured volume Bark, like wood, typically contains large amounts of water when fresh. In general, the bark of most species has weight to volume characteristics similar to the wood of the same species. In the UNECE region, the bark of conifers and non-coniferous species ranges from as little as 4% of the total over bark volume (and weight) to as much as 30%. Based on the questionnaire results shown in section 1.3, the percentage of bark averages about 11-12% of the over bark volume. Roundwood weight is normally reported with bark present; however, roundwood volume for UNECE/FAO purposes and many national roundwood measurement standards is reported for wood only, meaning that bark increases the weight to volume ratio of roundwood. Bark is an important source of forest-based energy, as well as having other uses such as decorative ground cover and soil treatment (mulch). Knowing the ratio of bark to roundwood volume is useful in terms of understanding weight ratios, but also for potential energy and other products that can be produced from bark. It is important to note, however, that bark volume typically decreases during handling from forest to mill, so the potential volume as reflected in over bark to under bark volumes are seldom available and highly volatile depending on log handling practices and season (bark loss from handling is generally higher during the spring of the year). Defects in roundwood, such as unsound fibre (decay), fractures, splits, crooked portions, etc., have weight, but often no volume, when the scaling method calls for a deduction, thus increasing the ratio of weight to volume for roundwood.
19 Forest products conversion factors for the UNECE Region Summary of country data on roundwood Czech Republic Finland France unit in/ Products unit out Saw/veneer logs Conifer Green weight with bark kg/m Wood basic density (dry weight/green m 3 ) kg/m Volume ratio wood/bark plus wood ub/ob Non-conifer Green weight with bark kg/m Wood basic density (dry weight/green m 3 ) kg/m Volume ratio wood/bark plus wood ub/ob Conifer and non-conifer Green weight with bark kg/m Wood basic density (dry weight/green m 3 ) kg/m Volume ratio wood/bark plus wood ub/ob National m 3 / true m 3 m 3 /m Pulp/fuelwood logs Conifer Green weight with bark kg/m Wood basic density (dry weight/green m 3 ) kg/m Volume ratio wood/bark plus wood ub/ob Non-conifer Green weight with bark kg/m Wood basic density (dry weight/green m 3 ) kg/m Volume ratio wood/bark plus wood ub/ob Conifer and non-conifer Green weight with bark kg/m Wood basic density (dry weight/green m 3 ) kg/m Volume ratio wood/bark plus wood ub/ob National m 3 / true m 3 m 3 /m Source: UNECE/FAO Forest Products Conversion Factor Questionnaire, Germany Ireland Netherlands Norway Slovakia Spain Sweden Switzerland United Kingdom United States Median Average
20 10 Forest products conversion factors for the UNECE Region 2. WOOD PARTICLES Wood particles (chips, sawdust, flakes and shavings), can be measured by volume or by weight (both in the dry state and as delivered ). All of these products start out as solid wood from logs of varying density, are broken down into somewhat irregular shaped particles, and often contain varied amounts of moisture and void space between the particles. Conversion factors for wood particles are determined by wood density, moisture content and compaction. In general, large enterprises that produce and use wood particles obtained from many sources, utilize oven dry weight as the unit of choice for measuring wood particles. Enterprises that work with wood particles obtained from fewer and more homogeneous sources might favour the use of volume or weight as delivered. Ultimately, the yield of most manufacturing processes using wood particles as a raw material is driven by the quantity of fibre excluding moisture and void. Another driver of the yield of wood particles is classification. Often users of wood particles require particles within certain size classifications for the product that they are manufacturing e.g. some pulping processes and OSB. A sawmill or wood-chipping operation may need to remove small particles (fines) from the on specification particles, which would result in a lower yield of chips but a higher yield of small particles, which may be classified and marketed as sawdust. 2.1 Volumetric measurement Procedures for establishing the volume of particles is straightforward. Volumes contained in truck-loads, ship-hulls and bins can be easily calculated. Even huge irregularly shaped stockpiles at manufacturing facilities can be measured with surveying equipment to establish volume. Solid wood equivalent is more complicated, however, as a result of the variation in void space. Wood particles in containers or piles will settle over time and the heavier the particles (due to density or moisture content) and the greater the depth (thus increasing weight), the more compaction will occur. Based on the data obtained from the questionnaire, the median volume of wood particles per cubic metres of solid wood was 2.83 m 3 for coniferous species (meaning that one cubic metre of solid wood will produce wood particles that displace 2.83 cubic metres including void space) and the median number for nonconiferous was 2.74 cubic metres. In Conversion Factors for the Pacific Northwest Forest Industry (Hartman et al, 1981), the following are listed as ratios of m 3 loose to m 3 solid for wood particles: pulp chips (compacted) 2.50 pulp chips (un-compacted) 2.86 sawdust 2.50 planer shavings Weight The weight of wood particles is generally reflected as delivered or as an oven dry weight (all moisture removed). The as delivered weight can have substantial variability as a result of the moisture content. For example: chips from a sawmill may have 50% mcw (50% of the weight is water and 50% is dry fibre), while a veneer plant, using identical logs for raw material as the sawmill, may produce chips where only 6% (mcw) of the weight is moisture. In this example, the sawmill chips were green, while the veneer chips would have been produced from dried veneer. Based on the questionnaire results, the median ratio of delivered metric tons to oven dried metric tons is 2.0 for conifers (indicating 50% dry fibre, 50% mcw) and 1.79 for non-coniferous (indicating 56% dry fibre and 44% mcw ).
10 March 2009 Page 1 FOREST PRODUCT CONVERSION FACTORS: PROJECT OVERVIEW AND STATUS 1. USE OF CONVERSION FACTORS 1.1 Background The term forest products conversion factors is used to cover a broad spectrum
PB 1650 Understanding Log Scales and Log Rules 1 Understanding Log Scales and Log Rules Brian Bond, Former Assistant Professor, Forestry, Wildlife and Fisheries Introduction A necessary step in determining
1 Chapter 3. Stacked Roundwood, Preservative-Treated Products, and Construction Logs Stacked Roundwood 38 Cord Measure 38 Standard rough cord Long cord The unit Face cord Volume of solid wood in a cord
What Do You See? FOR 274: Forest Measurements and Inventory Tree and Wood Volume Log Volumes Cords Weight Scaling Logs and Scaling: Definitions Logs: cut trees lengths of 8ft or more The process of measuring
Joint Session of the ECE Timber Committee and the FAO European Forestry Commission Location, Turkey 10 14 October 2011 Graphs Showing Forecasts made for 69th Timber Committee meeting (supplement) UNECE/FAO
211 Global Forest Products Facts and Figures FAO s forest product statistics present figures for the production and trade (quantity and value) of forest products, covering 52 product categories, 21 product
Global Wood Markets: Consumption, Production and Trade By Ed Pepke Forest Products Marketing Specialist UNECE/FAO Timber Section Geneva, Switzerland Presentation topics I. Introduction II. Where is the
InnovaWood/Wood Technology Institute Poznan, 25-26.06.2007 Wood market in Poland: structure of use, industrial and energy purposes Prof. Ewa Ratajczak, PhD Wojciech Cichy, PhD Joanna Pikul, MSc Wood Technology
Measuring Pulp Logs and Biomass: results of log studies Matt Fonseca UNECE/FAO Timber Section Measuring pulp logs and biomass What does the purchaser want? An accurate predictor of useable fiber What are
New Hampshire Native Lumber Law RSA 434-:59-61 Self Study Booklet Issued by: UNH Cooperative Extension 210 Nesmith Hall, 131 Main St. Durham, NH 03857 Contact: Sarah Smith (603)862-2647 email@example.com
ITEM 5 GLOBAL WOOD AND WOOD PRODUCTS FLOW TRENDS AND PERSPECTIVES Table of Contents GLOBAL WOOD AND WOOD PRODUCTS FLOW - TRENDS AND PERSPECTIVES... 1 SUMMARY... 2 INTRODUCTION... 3 INTERNATIONAL TRADE...
292 Vol. 6 FACTORS WHICH INFLUENCE COMPANIES IN FOREST MANAGEMENT DECISIONS B. D. McCONCHIE J. G. Groome and Associates, Taupo, New Zealand ABSTRACT Factors which generally influence companies in making
Country Report, SWEDEN Bo Hektor 1 & Erik Ling 2 1. Talloil AB, Klarabergsviadukten 70, D7, SE 111 64 Stockholm, Sweden, +46 70 6570043, Bo.Hektor@talloil.se 2. Sveaskog AB, 105 22 Stockholm, Sweden, +46
FOR 306 Forest measurements Trees eight weight Measure of the quantity of wood eight used also for: Scaling Complete tree utilization root, branches or stump Biomass Carbon content Fuel eight determined
A Log Volume Formula for Exporters J.C. Ellis Summary This paper shows that the volume estimate of export logs would be more accurate using a taper value in the 3D formula than volumes derived from the
Economic Parameters For Estimating the Delivered Wood Cost in the Deh Cho Planning Area Submitted by: John O Brien, Associate Kelvin Mak, Senior Manager, Forest Industry Team Leader 500 West Tower, 14310-111
North Central Forest Experiment Station 7.03 NTRAL HARDWOOD NOTES Grading Hardwood Trees Tree grading provides a way to evaluate the quality characteristics and value of standing hardwood trees. This is
EPPO Study on Wood Commodities Other than round wood, sawn wood and manufactured items Background Identification of different types of commodities + Bark + Isolated bark + Wood + Processed wood material
Wood fuel market development in Northern Europe EUBIONET2 - International training programme Lasse Okkonen North Karelia University of Applied Sciences Lasse.Okkonen@pkamk.fi Wood fuels in Europe Consumption
Introduction The purpose of this publication is to provide a simplified but thorough explanation of the grading rules for American hardwood lumber. They were established over 100 years ago by the newly
Smalian s Formula 4 November 1, 011 4-1 Scaling Manual Ministry of Forests, Lands and NRO 4.1 Smalian's Formula From the inception of cubic scaling the Smalian formula, which calculates logs on the basis
SCALING MANUAL Ministry of Natural Resources Prepared under the Authority of The Crown Forest Sustainability Act Third Edition April 1, 2007 ii Cette publication est également disponible en francais Printed
Wood Properties Technology T Practical Lesson Activity information Level: Junior secondary school Years 7 10 Duration: Preparation: Summary: Approximately 2 lessons Collect two samples of timber Students
United States Department of Agriculture Forest Service Pacific Northwest Forest and Range Experiment Station Research Paper PNW-337 May 1985 Comparison of Logging Residue from Lump Sum and Log Scale Timber
Agricultural Extension Service The University of Tennessee PB1693 Sawing Logs for Quartersawn Lumber 1 Table of Contents What Does Quartersawn Mean? 3 Planes of Reference 3 Terms Quartersawn and Plain-sawn
Timber Harvesting and Long-distance Transportation of Roundwood 214 Metsätehon tuloskalvosarja 7b/215 Markus Strandström Metsäteho Oy About statistics Includes volumes and direct harvesting costs of timber
United States Department of Agriculture Forest Service Forest Products Laboratory General Technical Report FPL-GTR-76 Specific Gravity, Moisture Content, and Density Relationship for Wood William T. Simpson
The Forest Industry: harvest, demand and foreign trade Timber Measurements Society Central Meeting April 10, 2014 Coeur d Alene, Idaho 2013 Forest2Market, Inc. 2 Forest2Market Data Experience Expertise
Catalogue no. 11-621-M, no. 89 ISSN 1707-0503 ISBN 978-1-100-19666-4..Analytical Paper... Analysis in Brief An Overview of the Lumber Industry in Canada, 2004 to 2010 by Benoit Germain Manufacturing and
Economic sustainability for wood pellets production A comparative study between Finland, Germany, Norway, Sweden and the US Erik Trømborg Co-authors: Geir Skjevrak,Tapio Ranta, Jörg Schweinle, Birger Solberg
ECE / FAO Forest Products Annual Market Review, 1998-1999 19 CHAPTER 3 ESTONIA S FOREST PRODUCTS MARKETS 1 Highlights The Estonian forestry sector has been characterized by rapid growth of foreign investments
SPECIFICATIONS FOR BRIDGE CONSTRUCTION SECTION 23 DIMENSIONAL STRUCTURAL LUMBER AND PILING TABLE OF CONTENTS 23.1 General...23-1 23.2 Standards...23-1 23.3 Material Specification...23-1 23.3.1 Planking
DIVISION OF AGRICULTURE R E S E A R C H & E X T E N S I O N University of Arkansas System Agriculture and Natural Resources FSA5015 Forest Landowner s Guide to Field Grading Hardwood Trees Kyle Cunningham
Forestry Terms Acre A land area of 43,560 square feet, approximately 209 ft. by 209 ft. Allowable cut The volume of wood that can be cut during a given period without exceeding the forest s net growth.
Tree Biomass & Carbon Price & Cost Information FOR 1001 Dr. Thom Erdle Today s Objectives Meaning and measurement of biomass and carbon Meaning and calculation of stumpage Familiarity with pricing cost
Valuing Timber Resource Stocks in the Canadian Natural Resource Stock Accounts London Group, November 2013 Environment Accounts and Statistics Division Statistics Canada October 18 th, 2013 Quick facts
APPEARANCE GRADES NOVEMBER 2012 This document contains information on the primary grades of appearance timber. Appearance grades of timber, rough or surfaced two faces, shall unless otherwise specified,
How Can We Measure Trees and Logs for more Useful Information For: Timber Measurement Society Coeur D Alene, Idaho April 12, 2012 By: Toby Atterbury Atterbury Consultants, Inc 3800 SW Cedar Hills Blvd.
LOGGING RATES PIEDMONT CUT & LOAD CONTRACT RATES US$ per Ton COASTAL PLAIN Harvest Type LO HI AVG Harvest Type LO HI AVG Final Harvest 10.22 14.67 12.44 Final Harvest 9.00 11.45 10.23 Plantation Thin 10.67
How is carbon stored in trees and wood products? Science S Theory Lesson Lesson information Level: Junior secondary school Year 10 Duration: Summary: Approximately 3 lessons Sustainably managed forests
FORECASTING AND MONITORING MOISTURE CONTENT OF WOODY BIOMASS IN IRELAND AND OREGON TO IMPROVE SUPPLY CHAIN ECONOMICS Glen Murphy 1, Francisca Belart 2, Tom Kent 3 and Pieter D. Kofman 4 ABSTRACT Wood is
The Dynamics of Global Pellet Markets Growth prospects and price scenarios Silvio Mergner Pöyry Management Consulting 4. Central European Biomass Conference 15-18 January 214 AGENDA Status Quo of the Industry
STEAM AND ELECTRICAL CONSUMPTION IN A COMMERCIAL SCALE LUMBER DRY KILN Tom Breiner and Stephen L. Quarles Forest Products Laboratory University of California Richmond, California Dean Huber U.S. Forest
Biomass availability and supply for co-firing projects in Alberta Dominik Roser, Ph.D. About FPInnovations A private non-profit Canadian corporation Supports competitiveness of the Canadian forest sector
Key Global Drivers & Impacts on the US Markets: Basis of a Super-Cycle COFI Annual Meeting, Prince George BC April 4, 2013 By: Russell Taylor, President 2a Introduction to: International WOOD MARKETS Group
Land areas and biomass production for current and future use in the Nordic and Baltic countries Lars Rytter The Forestry Research Institute of Sweden October 22, 2014 Skogforsk in brief Forestry and the
MODELLING AND PROJECTIONS OF WOOD PRODUCTS DEMAND, SUPPLY AND TRADE IN EUROPE Provisional description of the market modelling approach used for EFSOS II and EUwood, and some results Ragnar Jonsson, The
Hardwood Lumber Lesson Plan Keywords: hardwood, softwood, grading, dry-kiln, sawmill, and board foot Lesson Plan Grade Level: 6 th - 8 th Total Time Required For Lesson: 50 minutes (as one continuous time
NATIONAL GRADING RULE FOR SOFTWOOD DIMENSION LUMBER INTERPRETATIONS Index Part - National Grading Rule for Softwood Dimension Lumber Interpretations.. 5-9.0 General...5. Bark and Pitch Pockets...5.2 Bevel
Analysis of timber production and trade data in Central & Eastern Europe Timber Regulation Enforcement Exchange: Vienna Sep 16, 2015 Brief note on data sources FAO EU forest production data Eurostat: Main
Post and Beam Construction A Presentation By the Canadian Wood Council Canadian Conseil Wood canadien Council du bois Early settlers introduced the concept of post and beam construction in North America
1 ECONOMIC COMMISSION FOR EUROPE Timber Committee October 2014 FINLAND MARKET STATEMENT 1 GENERAL ECONOMIC TRENDS Along with the weak economic performance and sluggish demand in the euro area, the main
Dr. Thünen Institute of International Forestry and Forest Economics, Hamburg Second Meeting of the UNECE/FAO Team of Specialists on Wood Energy Slide Vienna, 1 11.- How much wood do we use? And what for?
Biomass Pellet Prices Drivers and Outlook What is the worst that can happen? European Biomass Power Generation 1st October 2012 Cormac O Carroll Director, London Office Pöyry Management Consulting (UK)
ENERGY VS. MATERIAL: USES OF WOOD BIOMASS - ECONOMIC IMPACTS OF ALTERNATIVE SCENARIOS Peter Schwarzbauer, Applied Life Vienna (Boku) and Tobias Stern, Competence Centre for Wood Composites and Wood Chemistry
UNSTAT TRADE DATA AS BASIS FOR ANALYSIS AND PROJECTION OF FOREST PRODUCTS TRADE FLOWS EFI Working Paper 17 Bruce Michie Philip Wardle 2 Bruce Michie and Philip Wardle EFI Working Paper 17 Authors Publisher
Timber Grading 8 November 1, 2011 8-1 Scaling Manual Ministry of Forests, Lands and NRO 8.1 Timber Grading Scaling under the Forest Act means to determine the volume and to classify the quality of timber.
Review of Canadian Apple Market & Trends 215 Mid-Summer Meeting- Canadian Apple Industry Wolfville, NS August 4 th, 215 Farid Makki Sector Development & Analysis Directorate Agriculture and Agri-Food Canada
Technologies and Economics of Energy Generation from Logging Residues and Wood Processing Waste Prof. Dr. Arno Frühwald University of Hamburg and Federal Research Centre for Forestry and Forest Products
5 2. Trade in forest commodities The volume of wood products in international trade increased 125 percent between 1992 and 2008 (FAO, 2010b). Some examples of the changes in volume of exports of particular
BIOMASS SOURCING STRATEGIES NON-TECHNICAL CHALLENGES OF A COMPANY INTENDING TO BUILD A DEMONSTRATION/FLAGSHIP PLANT EUROPEAN BIOFUELS TECHNOLOGY PLATFORM 5 TH STAKEHOLDER PLENARY MEETING 6 February 2013
Wood Ski Build Log Minnesota, Summer 2013 Basic Plans The basic plan for the skis are from an article in Fine Woodworking, Cross Country Skis, The Easy Way 1981 #31 The skis are two thin laminations of
Renewable Energy from Biomass Opportunities in London and Area? Eric Rosen KMW ENERGY INC. LONDON, ONTARIO Tel: (519) 686-1771 www.kmwenergy.com Company Background Long History in designing bioenergy systems.
CANADIAN MILL SERVICES ASSOCIATION CURRICULUM OF EDUCATION PROGRAMS ORGANIZATION HISTORY The formation of Canadian Mill Services Association came about in early 1994 after an indepth review and organization
,a! California State of California Department of Forestry, ~ The ResourcesAgency - ~A' ~;::~Af;// ~/ ~~/1Y~~,\~'(.~~~~~ ~,~ F1rl WES7:RY ~~~~_.~~- note 1416 Ninth Street Sacramento, CA 95814 Phone 916-445-5571
ORIENTED STRAND BOARD PART I. - GENERAL 1.1 RELATED DOCUMENTS A. Drawings and general provisions of Contract, including General and Supplementary Conditions and Division 1 Specification Sections, apply
MEASUREMENT Introduction: People created systems of measurement to address practical problems such as finding the distance between two places, finding the length, width or height of a building, finding
UNECE United Nations Economic Commission for Europe Food and Agriculture Organization of the United Nations GENEVA TIMBER AND FOREST DISCUSSION PAPER 42 FORESTS, WOOD AND ENERGY: POLICY INTERACTIONS Edited
BIOMASS SUPPLY CHAIN MANAGEMENT AND CONTROLLING FOCUS AND CONTENT The focus of the presentation is on forest biomass in Central Finland Content Entities of the forest biomass demand and supply chain Forest
FREQUENTLY ASKED QUESTIONS Biomass Harvest Guidelines What do Biomass Harvest Guidelines offer? They offer recommendations to manage forest-, brush- and open- land with the intent to protect water, timber,
Enova conference EKMAN & CO Trondheim January 25, 2012 This is Ekman Ekman is one of the world s leading sales and marketing organizations, focusing on the global forest industry. Business concept To add
R e q u e s t f o r Q u o t e s H a r d w o o d S w i t c h T i e s 15-15 2 0 1 3, 2 0 1 4, 2 0 1 5 C a p i t a l M a i n t e n a n c e P r o g r a m The Northern New England Passenger Rail Authority (NNEPRA),
for RGGI U.S. Forest Projects Outside of California, Oregon, Washington, Alaska and Hawaii May 13, 2015 Background on the Component Ratio Method... 2 Streamlined Approach to the Component Ratio Method...
Chapter 8. Pulp and Paper Pulp Yield 96 Mechanical Pulping 96 Chemical Pulping 96 Kraft (sulfate) process Sulfite process Hybrid Pulping Methods 97 Dissolving Pulp 97 Estimating Wood Required per Ton of
THE QUEBEC WOOD SUPPLY GAME: AN INNOVATIVE TOOL FOR KNOWLEDGE MANAGEMENT AND TRANSFER Constance VAN HORNE and Philippe MARIER FOR@C Research Consortium, Pavillon Pouliot, Université Laval, Quebec City,
CURLY BIRCH (Betula pendula var. carelica) AND ITS MANAGEMENT IN FINLAND Risto Hagqvist Finnish Forest Research Institute Haapastensyrjä Tree Breeding Station Karkkilantie 247, FIN-12600 Läyliäinen e-mail:
$2.50 PB1772 A Hardwood Log Grading Handbook Contents How Much Is a Log Worth?...1 Veneer, Sawlogs and Other Log Classes...2 Log Scaling...3 Table 1. The Doyle Log Rule...4 Log Grading Relation to Lumber